Journal of Hazardous Materials 177 (2010) 70–80
Contents lists available at ScienceDirect
Journal of Hazardous Materials journal homepage: www.elsevier.com/locate/jhazmat
Adsorption of methylene blue on low-cost adsorbents: A review Mohd. Rafatullah a,∗ , Othman Sulaiman a , Rokiah Hashim a , Anees Ahmad b a b
Division of Bioresource, Paper and Coatings Technology, School of Industrial Technology, Universiti Sains Malaysia, 11800 Penang, Malaysia Division of Environmental Technology, School of Industrial Technology, Universiti Sains Malaysia, 11800 Penang, Malaysia
a r t i c l e
i n f o
Article history: Received 25 June 2009 Received in revised form 23 October 2009 Accepted 8 December 2009 Available online 14 December 2009 Keywords: Adsorption Methylene blue Low-cost adsorbents Agricultural wastes
a b s t r a c t In this article, the use of low-cost adsorbents for the removal of methylene blue (MB) from solution has been reviewed. Adsorption techniques are widely used to remove certain classes of pollutants from waters, especially those which are not easily biodegradable. The removal of MB, as a pollutant, from waste waters of textile, paper, printing and other industries has been addressed by the researchers. Currently, a combination of biological treatment and adsorption on activated carbon is becoming more common for removal of dyes from wastewater. Although commercial activated carbon is a preferred adsorbent for color removal, its widespread use is restricted due to its relatively high cost which led to the researches on alternative non-conventional and low-cost adsorbents. The purpose of this review article is to organize the scattered available information on various aspects on a wide range of potentially low-cost adsorbents for MB removal. These include agricultural wastes, industrial solid wastes, biomass, clays minerals and zeolites. Agricultural waste materials being highly efﬁcient, low cost and renewable source of biomass can be exploited for MB remediation. It is evident from a literature survey of about 185 recently published papers that low-cost adsorbents have demonstrated outstanding removal capabilities for MB. © 2009 Elsevier B.V. All rights reserved.
Contents 1. 2.
Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Adsorbent literature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1. Activated carbon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2. Non-conventional low-cost adsorbents . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2.1. Natural materials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2.2. Bioadsorbents . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2.3. Waste materials and by-product from agriculture and industry . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2.4. Miscellaneous adsorbents . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Acknowledgement . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
1. Introduction The presence of dyes in efﬂuents is a major concern due to their adverse effects to many forms of life. The discharge of dyes in the environment is a matter of concern for both toxicological and esthetical reasons . Industries such as textile, leather, paper, plastics, etc., use dyes in order to colour their products and also
∗ Corresponding author. Tel.: +60 4 653 5219, fax: +60 4 657 3678. E-mail addresses: mohd [email protected]
, [email protected]
(Mohd. Rafatullah). 0304-3894/$ – see front matter © 2009 Elsevier B.V. All rights reserved. doi:10.1016/j.jhazmat.2009.12.047
70 71 71 72 72 73 74 76 76 77 77
consume substantial volumes of water. As a result, they generate a considerable amount of coloured wastewater . It is estimated that more than 100,000 commercially available dyes with over 7 × 105 tonnes of dyestuff produced annually [3–5]. It is recognized that public perception of water quality is greatly inﬂuenced by the colour. The colour is the ﬁrst contaminant to be recognized in wastewater. The presence of even very small amounts of dyes in water – less than 1 ppm for some dyes – is highly visible and undesirable [6,7]. MB is the most commonly used substance for dying cotton, wood and silk. It can cause eye burns which may be responsible for permanent injury to the eyes of human and animals. On inhalation, it can give rise to short periods of rapid or
Mohd. Rafatullah et al. / Journal of Hazardous Materials 177 (2010) 70–80
difﬁcult breathing while ingestion through the mouth produces a burning sensation and may cause nausea, vomiting, profuse sweating, mental confusion and methemoglobinemia [8–10]. Therefore, the treatment of efﬂuent containing such dye is of interest due to its harmful impacts on receiving waters. During the past three decades, several physical, chemical and biological decolorization methods have been reported; few, however, have been accepted by the paper and textile industries . Amongst the numerous techniques of dye removal, adsorption is the procedure of choice and gives the best results as it can be used to remove different types of coloring materials [12–14]. Recently, numerous approaches have been studied for the development of cheaper and effective adsorbents. Many non-conventional low-cost adsorbents, including natural materials, biosorbents, and waste materials from agriculture and industry, have been proposed by several workers. These materials could be used as adsorbents for the removal of dyes from solution. Many treatment processes have been applied for the removal of dyes from wastewater such as: photocatalytic degradation [15,16], sonochemical degradation , micellar enhanced ultraﬁltration , cation exchange membranes , electrochemical degradation , adsorption/precipitation processes , integrated chemical–biological degradation , integrated iron(III) photoassisted-biological treatment , solar photo-Fenton and biological processes , Fenton-biological treatment scheme  and adsorption on activated carbon [26,27]. As synthetic dyes in wastewater cannot be efﬁciently decolorized by traditional methods, the adsorption of synthetic dyes on inexpensive and efﬁcient solid supports was considered as a simple and economical method for their removal from water and wastewater . Methods of dye wastewater treatment have been reviewed by Pokhrel and Viraraghavan ; Robinson et al. ; Slokar and Majcen Le Marechal ; Delee et al. ; Banat et al. ; Cooper ; Crini  and Gupta and Suhas . Fungal and bacterial decolorization methods have been reviewed by Aksu ; Wesenberg et al. ; Pearce et al. ; McMullan et al. ; Fu and Viraraghavan  and Stolz . Adsorption is a well known equilibrium separation process and an effective method for water decontamination applications [39–42]. Adsorption has been found to be superior to other techniques for water re-use in terms of initial cost, ﬂexibility and simplicity of design, ease of operation and insensitivity to toxic pollutants. Adsorption also does not result in the formation of harmful substances. The present review article deals the technical feasibility of various non-conventional low-cost adsorbents for MB removal from water and wastewater. The main aim of this review is to provide a summary of recent information concerning the use of low-cost materials as adsorbents. For this, an extensive list of adsorbents literature has been compiled. The authors recommend that the reported adsorption capacities be taken as speciﬁc set of conditions rather than as maximum adsorption capacities. The reader is strongly encouraged to refer to the original research papers for information on experimental conditions.
2. Adsorbent literature 2.1. Activated carbon Though commercially available activated carbon (CAC) are usually derived from natural materials such as biomass, lignite or coal, but almost any carbonaceous materials may be used as precursor for the preparation of carbon adsorbents [43–52], because of its availability and cheapness, coal is the most commonly used precursor for activated carbon production. Coal is a mixture of car-
Table 1 Adsorption capacities for commercial activated carbon and coal. Adsorbents
Adsorption capacity (mg/g)
Commercial activated carbon Activated carbon produced from New Zealand coal Filtrasorb 400 Activated carbon Activated carbon produced from Venezuelan bituminous coal Peat Coal Filtrasorb 400 Norit Picacarb Filtrasorb 300 Activated carbon Coal Commercial activated carbon Bituminous coal Charcoal Activated carbon
476 400 380
  
324 323.68 299 276 246 240 238 230 200 176 62.7 9.81
           
bonaceous and mineral materials, resulting from the degradation of plants. The sorption properties of each individual coal are determined by the nature of the original vegetation and the extent of the physical–chemical changes occurring after deposition. Coal adsorption capacities are reported in Table 1. Coal based adsorbents have been used by Karaca et al. ; El Qada et al. ; Tamai et al. ; Banat et al.  and McKay et al. [56,57] with success for dye removal. However, since coal is not a pure material, it has a variety of surface properties and thus different sorption properties. Biomass and other waste materials may also offer an inexpensive and renewable additional source of activated carbon. These waste materials have little or no economic value and often present a disposal problem. Therefore, there is a need to valorize these low-cost by-products. So, their conversion into activated carbon would add economic value, help reduce the cost of waste disposal and most importantly provide a potentially inexpensive alternative to the existing commercial activated carbons. A wide variety of carbons have been prepared from biomass and other wastes, such as date pits , olive stones , furniture, sewage char and tyres [60,61], vermiculata plant , bamboo dust, coconut shell, groundnut shell, rice husk and straw [47,62], polyvilnyldieneﬂuoride ﬁbers , jute ﬁber , zeolite , coconut husk [9,54], oil palm ﬁber [66,67], waste apricot , corncob , coir pith , Pitch , olive-seed waste , ﬁr wood , rattan sawdust , bio-plant of Euphorbia rigida , vetiver roots , durian shell , oil palm shell , sugars , wheat bran , Hevea brasiliensis seed coat , peach stones , almond shell, walnut shell, hazelnut shell and apricot stones  and Rosa canina seeds . The excellent ability and economic promise of the activated carbons prepared from biomass exhibited high sorption properties as shown in Table 2. Kannan and Sundaram  reported the adsorption capacities of 472.10 mg/g of activated carbons made from straw. However, the adsorption capacities of carbons depend upon the sources of the raw materials used, the history of its preparation and treatment conditions such as pyrolysis temperature and activation time. Many other factors can also affect the adsorption capacity in the same sorption conditions such as surface chemistry (heteroatom content), surface charge and pore structure. A suitable carbon should possess not only a porous texture, but also high surface area. Recently, Guo et al.  showed that the adsorption does not always increase with surface area. Besides the physical structure, the adsorption capacity of a given carbon is strongly inﬂuenced by the chemical nature of the surface. The acid and
Mohd. Rafatullah et al. / Journal of Hazardous Materials 177 (2010) 70–80
Table 2 Adsorption capacities for activated carbons derived from agricultural and industrial wastes. Adsorbents
Adsorption capacity (mg/g)
Polyvilnyldieneﬂuoride activated carbon ﬁbers Straw activated carbon Bamboo based activated carbon Activated carbon (molasses/sulphuric acid) Activated carbon prepared from coconut husk Vetiver roots activated carbon-H2 O Peach stones based activated carbon Oil palm ﬁber-based activated carbon Mesoporous carbons prepared by using alkaline-treated zeolite Vetiver roots activated carbon-P1.5 Rice husk activated carbon HCl-treated oil palm shell-based activated carbon Rattan sawdust-activated carbon Activated carbon prepared from durian shell Coconut shell activated carbon Oil palm ﬁber-based activated carbon Olive-seed waste residue-based activated carbon Activated carbon prepared from oil palm shell Hevea brasiliensis seed coat-activated carbon Activated tyre char Jute ﬁber carbon Mesoporous carbons prepared by using acid-treated zeolite Activated furniture (850 ◦ C) Dehydrated wheat bran carbon Groundnut shell activated carbon Bamboo dust activated carbon Activated tyres (850 ◦ C) Chemically activated Salsola vermiculata plant Activated sewage char (800 ◦ C) Activated carbon prepared from a renewable bio-plant of Euphorbia rigida Waste apricot-based activated carbon Pyrolysed furniture Coconut husk based activated carbon Pyrolized Salsola vermiculata plant (PRSV) Pitch/Y(OiPr)3 Pitch/Y(naphthoate)3 Activated Rosa canina seeds (500 ◦ C) Pitch Activated olive stones with 40 wt.% ZnCl2 at 873 K in a nitrogen atmosphere Activated date pits (900 ◦ C) Activated olive stones with 40 wt.% ZnCl2 at 873 K Activated date pits (500 ◦ C) Hazelnut shell-activated carbon 750 ◦ C Coir pith carbon Apricot stones-activated carbon 750 ◦ C Walnut shell-activated carbon 750 ◦ C Almond shell-activated carbon 750 ◦ C Fir wood based activated carbon Corncob based activated carbon
486 472.10 454.20 435 434.78 423 412 400 380
        
375 343.50 303.03
  
294.12 289.26 277.90 277.78 190–263
    
243.90 227.27 227 225.64 223
    
200 185.2 164.90 143.20 130 130 120 109.98
       
102 80 66 53 52 49 47.2 33 22.1
        
12.9 8.82 5.87 4.11 3.53 1.33 1.21 0.84
       
base character of a carbon also inﬂuences the nature of the dye isotherms. The adsorption capacity depends also on the accessibility of the pollutants to the inner surface of the adsorbent, which depends on their sizes. The speciﬁc sorption mechanisms through which the adsorption of dyes takes place on these adsorbents are still not clear. This is because adsorption is a complicated process and depends on several interactions such as electrostatic and/or non-electrostatic (hydrophobic) interactions. Although much has been accomplished in terms of sorption properties and kinetics, much work is still necessary to identify the sorption mechanisms clearly .
2.2. Non-conventional low-cost adsorbents Activated carbon has been popular choice as an adsorbent for the removal of MB from wastewater but its high cost poses an economical problem. Therefore, there is a need for the development of low cost and easily available materials, which can be used more economically on large scale. Due to the problems mentioned above, research interest into the production of alternative adsorbents to replace the costly activated carbon has intensiﬁed in recent years. Attention has focused on various natural solid materials, which are able to remove MB from the contaminated wastewater at low cost. The cost is actually an important parameter for the comparison and selection of adsorbents. An adsorbent can be considered as low cost if it requires little processing and abundant in nature . It may also be deﬁned as a by-product or waste material from the industry and needs additional disposal cost. Certain waste products from industries and agricultural operations, natural materials and bioadsorbents represent potentially economical alternative adsorbents. Many of them have been tested and proposed for MB removal. 2.2.1. Natural materials 126.96.36.199. Clays. The clays are hydrous aluminosilicates broadly deﬁned as those minerals that make up the colloid fraction (<2 m) of soils, sediments, rocks and water  and may be composed of mixtures of ﬁne grained clay minerals and clay-sized crystals of other minerals such as quartz, carbonate and metal oxides. The clays invariably contain exchangeable ions on their surface and play important role in the environment by acting as a natural scavenger of pollutants by taking up cations and/or anions either through ion exchange or adsorption or both. The prominent ions found on clay surface are Ca2+ , Mg2+ , H+ , K+ , NH4 + , Na+ , and SO4 2− , Cl− , PO4 3− , NO3 − . These ions can be exchanged with other ions easily without affecting the structure of clay mineral . Natural clay minerals are well known and familiar to mankind from the earliest days of civilization. Because of their low cost, abundance in most continents of the world, high sorption properties and potential for ion exchange, clay materials are strong adsorbents. They possess layered structure and are considered as host materials for the adsorbates and counter ions. Vermiculite clay has the largest surface area and the highest cation exchange capacity. Its current market price (about US$ 0.04–0.12/kg) is considered to be about 20 times cheaper than that of activated carbon . In recent years, there has been an increasing interest in utilizing clay minerals such as bentonite, kaolinite, diatomite and Fuller’s earth for their capacity to adsorb not only inorganic ions but also organic molecules. In particular, interactions between MB and clay particles have been extensively studied [8,85–97]. The clay minerals exhibit a strong afﬁnity for MB (Table 3). The adsorption of MB on clay minerals is mainly dominated by ion-exchange processes. This means that the sorption capacity can vary strongly with pH. Al-Ghouti et al.  showed that the mechanism of adsorption of dye onto diatomite is due to physiosorption (depending on the particle size) and the presence of electrostatic interactions (depending on the pH used). Relatively good removal capabilities of clays to uptake MB has been demonstrated by many researchers. Bagane and Guiza  reported an adsorption capacity of 300 mg/g and suggested that clay is a good adsorbent for MB removal due to its high surface area. Almeida et al.  studied the removal of MB from synthetic wastewater by using as montmorillonite and described it as an efﬁcient adsorbent where the equilibrium was attained in less than 30 min. The adsorption of dyes on kaolinite was also studied by Ghosh and Bhattacharyya  and reported that its adsorption capacity can be improved by puriﬁcation and by treatment with
Mohd. Rafatullah et al. / Journal of Hazardous Materials 177 (2010) 70–80 Table 3 Adsorption capacities for natural materials. Adsorbents
Adsorption capacity (mg/g)
Clay Montmorillonite clay Bentonite Diatomite Perlite Diatomite (Jordon) Bentonite Spent activated clay Hexane-extracted spent bleaching earth Carbonised spent bleaching earth Fibrous clay minerals Pyrophyllite Zeolite Palygorskite Amorphous silica NaOH-treated pure kaolin NaOH-treated raw kaolin Pure kaolin Raw kaolin Zeolite Calcined pure kaolin Calcined raw kaolin Clay Glass wool
300 289.12 151–175 198 162.3 156.6 150 127.5 120.5 94.5 85 70.42 53.1 50.8 22.66 20.49 16.34 15.55 13.99 10.82 8.88 7.59 6.3 2.24
                       
NaOH solution. The removal performances of Fuller’s earth and commercial activated carbon for MB were compared by Atun et al. . They showed that the adsorption capacity is greater of Fuller’s earth than that of CAC. Moreover, Fuller’s earth is an interesting adsorbent since its average price is US$ 0.04/kg whereas CAC costs US$ 20/kg. Shawabkeh and Tutunji  studied the adsorption of MB onto diatomaceous earth (diatomite). They showed that this naturally occurring material could substitute for activated carbon as an adsorbent due to its easy availability, low cost, and good sorption properties. Further, its adsorption isotherms revealed that adsorption equilibrium was reached within 10 min. The feasibility of using diatomite for the removal of the problematic reactive dyes was also investigated by Al-Ghouti et al. . The results presented above show that clay materials may be promising adsorbents from environmental and puriﬁcation point of views. 188.8.131.52. Zeolites and other siliceous materials. The siliceous materials such as perlite, glass and zeolites have been proposed for MB dye removal (Table 3). The use of natural siliceous adsorbents such as silica, glass ﬁbers and perlite for waste water is increasing because of their high abundance, easy availability and low cost. Among inorganic materials, amorphous silica deserves particular attention , considering chemical reactivity of their hydrophilic surface, resulting from the presence of silanol groups. Their porous texture, high surface area and mechanical stability also make them attractive as adsorbents for decontamination applications. However, due to their low resistance toward alkaline solutions their usage is limited to media of pH less than 8 . Moreover, the surface of siliceous materials contains acidic silanol (among other surface groups) which causes a strong and often irreversible nonspeciﬁc adsorption. Perlite is a glassy volcanic rock and has high silica content, usually greater than 70%. It is inexpensive and easily available in many countries. The use of perlite as a low-cost adsorbent for the removal of MB has been investigated by Dogan et al. [100,101]. It was suggested that MB is physically adsorbed onto the perlite. Thus perlite is a good adsorbent for decontamination purposes. However, perlites of different types (expanded and unexpanded) and of different origins have different properties because of the differences in composition. Chakrabarti and Dutta
 investigated the glass ﬁber for the adsorption of MB. They stated that a considerable amount of the dye is adsorbed on soft glass even at ambient temperature. Zeolites are highly porous aluminosilicates with different cavity structures. They consist of a three dimensional framework, having a negatively charged lattice. The electro neutrality is maintained by exchangeable counter ions. The characteristics and applications of zeolites have been reviewed by Ghobarkar et al. . High ion-exchange capacity and relatively high speciﬁc surface areas, and more importantly their relatively cheap prices, make zeolites more attractive adsorbents. Their price is about US$ 0.03–0.12/kg, depending on the quality of the mineral . Another advantage of zeolites over resins is their ion selectivities generated by their rigid porous structures. Woolard et al. , converted ﬂy ash into zeolitic products by the hydrothermal treatment of raw ash with base. The product was found to bear signiﬁcantly increased surface area and cation exchange capacity in comparison to the raw ash. This product also shows increased afﬁnity for sorption of cationic dyes when compared to the raw ash. It is, however, that this increase in sorption capacity is merely the result of the increase in surface area, rather than a speciﬁc interaction. Although the removal efﬁciency of zeolites for dyes may not be as good as that of clay materials, their easy availability and low cost may compensate for the associated drawbacks. 2.2.2. Bioadsorbents The accumulation and concentration of dyes from aqueous solutions by the use of biological materials is termed bioadsorption. In this instance, biomass used as an adsorbents in order to concentrate and to remove MB dye from solutions. The bioadsorbents are often much more selective than traditional ion-exchange resins and commercial activated carbons, and can reduce dye concentration to ppb levels. Bioadsorption is a novel approach, competitive, effective and cheap. 184.108.40.206. Biomass (dead and living). Removal of MB dye by biomass (dead or living), fungi, algae and other microbial cultures was the subject of many recent researches. It has been found that bioadsorbents derived from suitable algal biomass can be used for the effective removal of MB from aqueous solutions. The use of biomass for wastewater is increasing because of its availability in large quantities at low cost. Biomass has a high potential as an adsorbent due to its physico-chemical characteristics. Recent literature on the methods of removal of MB from wastewater focuses on MB adsorption [52,104–119]. Table 4 shows some of the adsorption capacities reported in the literature. Yu et al.  studied the poly (methacrylic acid) modiﬁed biomass of baker’s yeast to improve the adsorption capacity of MB. He also studied the poly(amic acid)-modiﬁed biomass of baker’s yeast to improve the adsorption capacities for removal of MB. Experimental results showed that pH and ionic strength had little effect on the capacity of the modiﬁed biomass, indicating that the modiﬁed biomass had good potential for practical use. According to the Langmuir equation, the maximum uptake capacities for MB were 869.6 mg/g for poly(methacrylic acid) modiﬁed biomass of baker’s yeast and 680.3 mg/g for poly(amic acid)-modiﬁed biomass of baker’s yeast respectively, which were 17 and 13 fold than that obtained on the unmodiﬁed biomass. Fu and Viraraghavan , demonstrated that in comparison with commercial activated carbon dead fungal biomass of Aspergillus niger is a promising biosorbents for MB dye removal. Waranusantigul et al.  also reported the usefulness of biomass for the removal of MB. The biosorption capacity of fungal biomass could be increased by some pretreatment (by autoclaving or by reacting with chemicals). In spite of good sorption properties and high selectivity some problems might occur. The sorption process
Mohd. Rafatullah et al. / Journal of Hazardous Materials 177 (2010) 70–80
Table 4 Adsorption capacities for bioadsorbents. Adsorbents
Poly(methacrylic acid) modiﬁed biomass of baker’s yeast Poly(amic acid) modiﬁed biomass of baker’s yeast Caulerpa lentillifera Alga Sargassum muticum seaweed Enteromorpha spp. Activated sludge biomass Dead macro fungi (Fomes fomentarius) Dead macrofungi (Phellinus igniarius) Hydrilla verticillata Moss Algae Gelidium Duckweed (Spirodela polyrrhiza) (at pH 9) Water hyacinth root Duckweed (Spirodela polyrrhiza) (at pH 7) Algal waste Composite material Unmodiﬁed biomass of baker’s yeast Green alga Ulva lactuca The brown alga Cystoseira barbatula Kutzing Dead Streptomyces rimosus Dead fungus Aspergillus niger Posidonia oceanica (L.) ﬁbres Caulerpa racemosa var. cylindracea Living biomass
Adsorption capacity (mg/g)
417 279.2 274 256.41 232.73 204.38 198 185 171 144.93 128.9 119 104 74 51.5 40.2 38.61 34.34 18.54 5.56 5.23 1.17
              [104,105]       
is slow and in case of biomass of Aspergillus niger the equilibrium was reached in 42 h. Another problem is that the initial pH of the dye solution strongly inﬂuenced the bioadsorption. Marungrueng and Pavasant  investigated the adsorption of MB onto green macro alga Caulerpa lentillifera. The results were compared to the sorption performance of a commercial activated carbon. The results revealed that the alga exhibited greater sorption capacities than activated carbon for the MB investigated in this work. For the sorption of MB, both alga and carbon seemed to have the same sorption rate. The sorption processes were initially controlled by both ﬁlm and pore-diffusion, and only were limited by pore diffusion in the later stage. The isotherms followed Langmuir model which suggested that the sorption was monolayer coverage. Maximum sorption capacity obtained from the sorption of MB onto C. lentillifera was 417 mg/g which was relatively higher in comparison with the previous records as summarized in Table 4. MB adsorption on Sargassum muticum, an invasive macro alga in Europe, has been investigated by Rubin et al.  using visible absorption spectroscopy. Different pre-treatments, protonation and chemical cross-linking with CaCl2 or H2 CO, have been tested in order to improve the stability as well as the adsorption capacity of the algal biomass. The equilibrium binding has been described in terms of Langmuir and Freundlich isotherms, depending on the biomass pre-treatment. It is remarkable that the percentage of MB removed is up to 90%, which is higher than that found for other biosorbents and it could be even compared with that of activated carbon (99.8% uptake). Bioadsorption kinetics has been described by means of the ﬁrst order Lagergren equation, from which the corresponding kinetics parameters were obtained. Nacera and Aicha  investigated the biosorption of basic dye, methylene blue onto dead Streptomyces rimosus. The results show the percentage of dye sorption increases with the increase in quantity of the dead bacterial biomass and reaches to highest value at 20 ◦ C. The bioadsorption capacity decreased from 9.86 to 6.93 mg/g with an increase in temperature from 20 to 50 ◦ C at the initial MB concentration of 50 mg/l. The kinetics of MB sorption by pre-treated dead S. rimosus were fast, reaching 86% (C0 = 50 mg/L) of the total adsorption capacity in 5 min. The mechanism follows a pseudo-second order
reaction model. The activation energy of sorption was evaluated as −7.18 kJ mol−1 and thus the process is exothermic. El-Khaiary  studied the adsorption characteristics of MB onto nitric-acid treated water-hyacinth (N-WH). The results showed that N-WH can remove MB effectively from aqueous solution. A complete removal of MB from solution was only achieved at the lower range of initial MB concentration (less than 286 mg/L). The amount of dye uptake (mg/g) was found to increase with the increase in contact time and initial MB concentration, but there is no linear relationship between the dye uptake and temperature. Laboratory investigations of the potential of the biomass of dried roots of water hyacinth (Eichhornia crassipes) to remove MB from aqueous solutions were studied by Low et al. . Removal of MB by invasive marine seaweed: Caulerpa racemosa var. cylindracea was studied by Cengiz and Cavas . The adsorption reached equilibrium at 90 min. for all studied concentrations (5–100 mg/L). Langmuir and Freundlich models were applied to the data related to adsorption isotherm. According to Langmuir model data, the observed maximum adsorption capacity was 5.23 mg/g at 18 ◦ C. The enthalpy of adsorption was found to be 33 kJ/mol, which indicated a chemical adsorption between MB molecules and C. racemosa var. cylindracea functional groups. Bio-adsorption processes are particularly suitable for the treatment of solutions containing dilute MB concentration. Biosorption is a promising potential alternative to conventional processes for the removal of MB [37,115]. However, these technologies are still in the developing stage and much more work is required. 2.2.3. Waste materials and by-product from agriculture and industry The waste materials and by-products from the agriculture and other industries could be assumed to be the low-cost adsorbents due to their abundance in nature and less processing requirements. 220.127.116.11. Agricultural solid wastes. The raw agricultural solid wastes such as leaves, ﬁbers, fruits peels, seeds etc. and waste materials from forest industries such as sawdust, bark etc. have been used as adsorbents. These materials are available in large quantities and may be potential adsorbents due to their physico-chemical characteristics and low cost. Sawdust is an abundant by-product of the wood industry that is either used as solid fuel for cooking or as packing material. Sawdust is easily available at the countryside at zero or negligible price . It contains various organic compounds (lignin, cellulose and hemicellulose) with polyphenolic groups that might be useful for binding MB through different mechanisms. The role of sawdust materials in the removal of pollutants from aqueous solutions has been reviewed recently  and some valuable guidelines can be drawn from the review. Sawdust has proven to be a promising low-cost material for the removal of MB from wastewater. Hamdaoui  studied the removal of MB, from aqueous solution (40 mg/L) onto cedar sawdust in order to explore their potential use as low-cost adsorbents for wastewater dye removal. Adsorption isotherms were determined at 20 ◦ C and the experimental data obtained were modelled with the Langmuir, Freundlich, Elovich and Temkin isotherm equations. By considering the experimental results and adsorption models applied in this study, it can be concluded that equilibrium data were represented well by a Langmuir isotherm equation with maximum adsorption capacity of 142.36 mg/g for cedar sawdust. The extent of the dye removal decreased with increase in the solution temperature and optimum pH value for dye adsorption was observed at pH 7 for both adsorbents. Ahmad et al.  investigated the scavenging behaviour of meranti sawdust in the removal of MB from aqueous solution. Batch studies were performed to evaluate and optimize the effects of various parameters such as contact time, pH, initial
Mohd. Rafatullah et al. / Journal of Hazardous Materials 177 (2010) 70–80
dye concentrations and adsorbent dosage. Langmuir, Freundlich and Temkin isotherms were used to analyze the equilibrium data at different temperatures. Equilibrium data ﬁtted very well in the Langmuir isotherm equation, conﬁrming the monolayer adsorption (120.48 mg/g) of MB onto meranti sawdust. Most of the studies showed that sawdust is natural form or modiﬁed form is highly efﬁcient for the removal of MB [125–129]. The summary of these research works is given in Table 5. Chemical pretreatment of sawdust has been shown to improve the adsorption capacity and to enhance the efﬁciency of sawdust adsorption [121,130–132]. Batzias and Sidiras  studied that beech saw dust as low-cost adsorbent for the removal of MB. Further, in order to know the effect of chemical treatment and to improve its efﬁciency the authors also tested the potential of the adsorbent by treating it with CaCl2 , using mild acid hydrolysis  and found it to increase the adsorption capacity. Besides this, the simulation studies for effect of pH were also carried out by Batzias and Sidiras . The authors determined the point of zero charge (pHzpc = 5.2) of the sawdust and suggested that increase of the pH enhances the adsorption behaviour. The low adsorption of MB at acidic pH was suggested to be due to the presence of excess H+ ions that compete with the dye cation for adsorption sites. With the increase of the pH of the system, the number of positively charged sites decreases while the number of the negatively charged sites increases that favour the adsorption of MB due to electrostatic attraction. Another waste product from the timber industry is bark, a polyphenol-rich material. Bark is an abundant forest residue which has been found to be effective in removing dyes from water solutions. Because of its low cost and high availability, bark is very attractive as an adsorbent. Like sawdust, the cost of forest wastes is only associated with the transport cost from the storage place to the site where they will be utilized. Bark is an effective adsorbent because of its high tannin content. Mckay et al.  used the teak wood bark as an adsorbent to remove the MB from aqueous solutions. Equilibrium isotherms were studied at 20 ◦ C using sealed ﬂasks in a temperature controlled, agitated shaker bath. A constant ﬁxed mass of adsorbent was shaken with 0.050 dm3 dye solution using solutions varying in dye concentration from 10 to 1000 ppm. Dynamic ﬂow studies were performed using glass columns, 0.010 m diameter and 0.150 m packed bed height, were used to determine the adsorption breakthrough curves. The dye solution ﬂow rates through the columns were maintained at 0.120 dm3 h−1 and 0.005 dm3 samples were collected for analysis out of every 0.100 dm3 of solution treated. The monolayer saturation capacity for MB onto teak wood bark is 914.59 mg g−1 . Rice husk is an agricultural waste and a by-product of the rice milling industry to be about more than 100 million tonnes, 96% of which is generated in the developing countries. The utilization of this source of agricultural waste would solve both a disposal problem as well as access to a cheaper material for adsorption in water pollutants control system . The maximum cost of commercially available rice husk is approximately US$ 0.025/kg. Since, the main components of rice husk are carbon and silica (15–22% SiO2 in hydrated amorphous form like silica gel), it has the potential to be used as an adsorbent. Mckay et al. [56,57] studied the use of rice husk in the removal of MB from aqueous solutions then after Vadivelan and Kumar  used the rice husk for the adsorption of MB. The operating variables studied were initial solution pH, initial dye concentration, adsorbent concentration, and contact time. The amount of dye adsorbed was found to vary with initial solution pH, adsorbent dose, and contact time. The monolayer sorption capacity of rice husks for MB sorption was found to be 40.58 mg/g at room temperature (32 ◦ C). The dye uptake process was found to be controlled by external mass transfer initially followed by intraparticle diffusion.
Table 5 Adsorption capacities for agricultural solid wastes. Adsorbents
Teak wood bark Papaya seeds Grass waste Pomelo (Citrus grandis) peel Rice husk Untreated guava leaves Jackfruit peel Cotton waste Banana stalk waste Palm kernel ﬁber Modiﬁed rice straw Broad bean peels Gulmohar (Delonix regia) plant leaf powder Castor seed shell Cedar sawdust Pumpkin seed hull Saw dust Chemically treated guava leaves Meranti sawdust Pineapple stem Dehydrated peanut hull Coconut husk Coffee husks Phosphoric acid treated Parthenium hysterophorus Teak wood bark Garlic peel Rubber seed shell Fallen phoenix tree’s leaves Raw date pits Ground hazelnut shells Coconut bunch waste Peanut hull Walnut sawdust Luffa cylindrica ﬁbers Yellow passion fruit waste Olive pomace Rice husk Cherry sawdust Sulphuric acid treated Parthenium hysterophorus Hazelnut shell Mansonia wood sawdust Modiﬁed sawdust Paspalum notatum (garden grass) Oak sawdust Rice husk Pitch-pine sawdust Cotton waste Salsola vermiculata leaves Jute processing waste Banana peel Cereal chaff Orange peel Spruce wood shavings from Picea abies Wheat shells Beech sawdust pretreated with 20% (w/v) CaCl2 for 1 h at 100 ◦ C Beech sawdust pretreated with 20% (w/v) CaCl2 for 1 h at 23 ◦ C Indian Rosewood sawdust Raw beech sawdust Coarse grinded wheat straw Neem (Azadirachta indica) leaf powder Fine grinded wheat straw
Adsorption capacity (mg/g)
914.59 555.55 457.64 344.83 312.26 295 285.71 277.77 243.90 217.95 208.33 192.72 186.22
            
158.73 142.36 141.92 133.87 133.33 120.48 119.05 108.6 99 90.1 88.49
          
84 82.64 82.64 80.9 80.3 76.9 70.92 68.03 59.17 47 44.70 42.3 40.59 39.84 39.68
              
38.22 33.44 32.3 30.4 29.94 28 27.78 24 23 22.47 20.8 20.3 18.6 17.91 16.56 16.05
               [130–132]
11.8 9.78 3.82 3.67 2.23
    
Mohd. Rafatullah et al. / Journal of Hazardous Materials 177 (2010) 70–80 Table 7 Adsorption capacities for miscellaneous type of adsorbents.
Table 6 Adsorption capacities for industrial solid wastes. Adsorbents
Adsorption capacity (mg/g)
Adsorption capacity (mg/g)
Activated sludge biomass Baggase bottom ash Sewage sludge from an urban wastewater Sewage sludge from an agrifood industry Coal ﬂy ash (0.01 NaCl) Coal ﬂy ash HNO3 Fly ash Fly ash (bagasse) Fly ash (CFA) Fly ash Fly ash Fly ash Fly ash Fly ash Red mud Fly ash (SFA) Fly ash Chrome sludge
256.41 142.54 114.9
  
Spent tea leaves Hair Crushed brick Tea waste Carbinized press mud Fe(III)/Cr(III) hydroxide Melamine–formaldehyde–urea resin Cow dung ash
300.05 120 96.61 85.16 50 22.8 15 5.31
       
16.6 12.7 7.99 6.46 6.04 5.57 4.60 4.47 3.07 2.85 2.49 1.47 1.10 0.51
             
Other agricultural solid wastes from cheap and readily available resources such as papaya seeds , grass waste [136,137], pomelo (Citrus grandis) peel , guava leaves [139,140], gulmohar (Delonix regia) plant leaf powder , jackfruit peel , cotton waste [56,57], banana waste [143,144], palm kernel ﬁber , rice straw , broad bean peels , rubber seed shell , castor seed shell , pumpkin seed hull , pineapple stem , dehydrated peanut hull , coconut husk , coffee husks , Parthenium hysterophorus , garlic peel , fallen phoenix tree’s leaves , raw date pits , ground hazelnut shells [126,158,159], coconut bunch waste , peanut hull , Luffa cylindrica ﬁbers , yellow passion fruit waste , olive pomace , Salsola vermiculata (SV) leaves , jute waste , cereal chaff , orange peel , wheat shells , wheat straw , neem (Azadirachta indica) leaf powder  have also been successfully employed for the removal of MB from aqueous solutions (Table 5). 18.104.22.168. Industrial solid wastes. Industrial solid wastes such as sludge, ﬂy ash and red mud are classiﬁed as low-cost materials because of their low cost and local availability and can be used as adsorbents for MB dye removal [107,169–176]. The activated sludge biomass collected from electroplating industry of Adana Organize Sanayi, Turkey was used as an adsorbent for MB by Gulnaz et al. . It contains insoluble metal hydroxides and other salts and showed the highest dye uptake capacity, having the monolayer adsorption capacity 256.41 mg/g for MB, at pH value of 7.0 and 20 ◦ C. Otero et al.  investigated the use of dried sewage sludges, pyrolysed sewage sludges and both chemically activated and pyrolysed sewage sludges as adsorbents material in single batch liquid-phase adsorption tests. The adsorption equilibriums of MB by these materials have been described in terms of both Langmuir and Freundlich equations. Among the various adsorbents used for removal of MB dye the ﬂy ash was found to be an effective adsorbent. Table 6 summarizes the adsorption capacity of MB onto the ﬂy ash. It is a waste/byproduct of thermal power plants and generally available free of cost that may be used in construction of roads, bricks and cement etc. Owing to its high availability and problem of disposal, a number of workers have attempted to use it as an adsorbent in pollution control. Although it may contain some hazardous substances, such as heavy metals, it is widely utilized in industry in many countries .
Eggshell and eggshell membrane polyacrylic acid-bound iron oxide magnetic nanoparticles
However, bagasse ﬂy ash generated in the sugar industry does not contain large amounts of toxic metals and has been widely used for adsorption of dyes . Fly ash has a surface area of 15.6 m2 /g . Its properties are extremely variable and depend strongly on its origin [171,175]. Wang et al.  used ﬂy ash as adsorbent for the removal of MB from aqueous solutions and the adsorption capacity for raw ﬂy ash was reported to be 4.47 mg/g. The effect of physical (heat) and chemical treatment was also studied on as-received ﬂy ash and the heat treatment was reported to have adverse effect on the adsorption capacity of ﬂy ash but acid treatment (by nitric acid) resulted in an increase of adsorption capacity of ﬂy ash (7.99 mg/g). Coal ﬂy ash was used successfully as low-cost adsorbents for removal of MB from aqueous solution by Wang et al. . Viraraghavan and Ramakrishna  investigated the use of coal ﬂy ash from the Shand power plant in Canada for removal of dyes from wastewater. The negative values of free energies indicate the feasibility and spontaneous nature of the process, and the positive heats of enthalpy suggest the endothermic nature of the process. Another abundant industrial by-product/waste material is red mud. Waste red mud is a bauxite processing residue discarded in alumina production. Red mud, an aluminum industry waste was converted into a low-cost potential adsorbent and the ﬁnal material has been used for the removal of MB by Wang et al.  who showed that physical and chemical treatment can signiﬁcantly change its adsorption capacity. 2.2.4. Miscellaneous adsorbents Various other materials have also been put to use for preparing alternative adsorbents. An attempt to remove MB by using waste tea leaves was studied by Uddin et al.  and Hameed , so as to develop a low-cost methodology while having low impact on environment. Besides this various other materials have also been studied less extensively as low-cost adsorbents, such as sand , stainless steel , hair , crushed brick , carbinized press mud , Fe(III)/Cr(III) hydroxide , melamine–formaldehyde–urea resin , cow dung ash , eggshell and eggshell membrane  and polyacrylic acid-bound iron oxide magnetic nanoparticles  have also been explored as an adsorbents. The adsorption capacities of these materials are given in Table 7. 3. Conclusions This review has attempted to cover a wide range of nonconventional low-cost adsorbents so that the reader can get an idea about the various types of low-cost materials used for the removal of MB from the wastewater. Inexpensive, locally available and effective materials could be used in place of commercial activated carbon for the removal of MB from aqueous solution. Little efforts
Mohd. Rafatullah et al. / Journal of Hazardous Materials 177 (2010) 70–80
seem to have been made to carry out a cost comparison between activated carbon and various non-conventional adsorbents. This aspect needs to be investigated further in order to promote largescale use of non-conventional adsorbents. In spite of the scarcity of consistent cost information, the widespread uses of low-cost adsorbents in industries for wastewater treatment applications today are strongly recommended due to their local availability, technical feasibility, engineering applicability, and cost effectiveness. If lowcost adsorbents perform well in removing MB at low cost, they can be adopted and widely used in industries not only to minimize cost inefﬁciency, but also improve proﬁtability. Undoubtedly lowcost adsorbents offer a lot of promising beneﬁts for commercial purposes in the future. Literature also reveals that in some cases the modiﬁcation of the adsorbent increased the removal efﬁciency. However, very less work has been carried out in this direction especially to understand the mechanism of adsorption. We speculate the possibility of the ion exchange mechanism to play an important role in MB uptake being a cationic dye. The following observations of different authors hint toward this mechanism: 1. Increase of adsorption capacity of CaCl2 treated adsorbents. 2. In crease of adsorption capacity in basic medium. 3. Decrease of adsorption capacity in acidic medium. In all these cases the ion exchange sites on the surface of adsorbents are converted to cationic form and cations are exchanged with MB, being a cationic dye, in the equilibrating solution. However, release of H+ ions (in the 3rd case) decreases pH of the solution and the condition becomes unfavourable for dye uptake by ion exchange and ultimately apparent total adsorption capacity decreases. Thus uptake of MB is accompanied by dual mechanism of ion exchange as well as adsorption. The process of bioadsorption requires further investigation in the direction of modeling, regeneration of bioadsorbents and recovery of MB and immobilization of the waste material for enhanced efﬁciency and recovery. Most of the reported studies are performed in the batch process; this gives a platform for the designing of the continuous ﬂow systems with industrial applications at the commercial level also. Further research is to be carried out to make the process economically viable at industrial scale with focus on MB recovery and regeneration of agricultural waste. Finally we wish to comment of zero waste strategy of adsorption process in treatment of water waste waters. There is a bigger scope of research of utilization of used adsorbents for further treatment processes. For example MB adsorbed adsorbents can further be explored for their application in second stage adsorption which is completely an unexplored area of research. Another possibility of exploration is the recovery cum reuse of adsorbed substances. All future researches might be accompanied by adsorption/desorption and/or adsorption/readsorption process so that there is no net sludge generation and, if any, it should be minimum. Such a strategy will fulﬁll the goal of zero waste. Acknowledgement One of the authors (M. Rafatullah) is grateful to the University Sains Malaysia, for providing assistance under the post doctoral scheme for this work. References  H. Metivier-Pignon, C. Faur-Brasquet, P.L. Cloirec, Adsorption of dyes onto activated carbon cloths: approach of adsorption mechanisms and coupling of ACC with ultra ﬁltration to treat coloured wastewaters, Sep. Purif. Technol. 31 (2003) 3–11.
 K. Ravi, B. Deebika, K. Balu, Decolourization of aqueous dye solutions by a novel adsorbent: application of statistical designs and surface plots for the optimization and regression analysis, J. Hazard. Mater. B122 (2005) 75–83.  G. McMullan, C. Meehan, A. Conneely, N. Kirby, T. Robinson, P. Nigam, I.M. Banat, R. Marchant, W.F. Smyth, Microbial decolourisation and degradation of textiles dyes, Appl. Microbiol. Biotechnol. 56 (2001) 81–87.  C.I. Pearce, J.R. Lloyd, J.T. Guthrie, The removal of colour from textiles wastewater using whole bacterial cells: a review, Dyes Pigments 58 (2003) 179–196.  J.W. Lee, S.P. Choi, R. Thiruvenkatachari, W.G. Shim, H. Moon, Evaluation of the performance of adsorption and coagulation processes for the maximum removal of reactive dyes, Dyes Pigments 69 (2006) 196–203.  T. Robinson, G. McMullan, R. Marchant, P. Nigam, Remediation of dyes in textiles efﬂuent: a critical review on current treatment technologies with a proposed alternative, Biresour. Technol. 77 (2001) 247–255.  I.M. Banat, P. Nigam, D. Singh, R. Marchant, Microbial decolourization of textile-dye-containing efﬂuents: a review, Bioresour. Technol. 58 (1996) 217–227.  D. Ghosh, K.G. Bhattacharyya, Adsorption of methylene blue on kaolinite, Appl. Clay Sci. 20 (2002) 295–300.  I.A.W. Tan, A.L. Ahmad, B.H. Hameed, Adsorption of basic dye on high-surfacearea activated carbon prepared from coconut husk: equilibrium, kinetic and thermodynamic studies, J. Hazard. Mater. 154 (2008) 337–346.  I.A.W. Tan, A.L. Ahmad, B.H. Hameed, Adsorption of basic dye using activated carbon prepared from oil palm shell: batch and ﬁxed bed studies, Desalination 225 (2008) 13–28.  S.M. Ghoreishi, R. Haghighi, Chemical catalytic reaction and biological oxidation for treatment of non-biodegradable textile efﬂuent, Chem. Eng. J. 95 (2003) 163–169.  A.K. Jain, V.K. Gupta, A. Bhatnagar, Suhas, Utilization of industrial waste products as adsorbents for the removal of dyes, J. Hazard. Mater. B101 (2003) 31–42.  Y.S. Ho, G. McKay, Sorption of dyes and copper ions onto biosorbents, Process Biochem. 38 (2003) 1047–1061.  F. Derbyshire, M. Jagtoyen, R. Andrews, A. Rao, I. Martin-Gullon, E. Grulke, Carbon materials in environmental applications, in: L.R. Radovic (Ed.), Chemistry and Physics of Carbon, vol. 27, Marcel Dekker, New York, 2001, pp. 1–66.  M.R. Sohrabi, M. Ghavami, Photocatalytic degradation of Direct Red 23 dye using UV/TiO2 : effect of operational parameters, J. Hazard. Mater. 153 (2008) 1235–1239.  M. Sleiman, D.L. Vildozo, C. Ferronato, J.M. Chovelon, Photocatalytic degradation of azo dye Metanil Yellow: optimization and kinetic modeling using a chemometric approach, Appl. Catal. B 77 (2007) 1–11.  M. Abbasi, N.R. Asl, Sonochemical degradation of Basic Blue 41 dye assisted by nanoTiO2 and H2 O2 , J. Hazard. Mater. 153 (2008) 942–947.  N. Zaghbani, A. Haﬁane, M. Dhahbi, Removal of Safranin T from wastewater using micellar enhanced ultraﬁltration, Desalination 222 (2008) 348–356.  J.S. Wu, C.H. Liu, K.H. Chu, S.Y. Suen, Removal of cationic dye methyl violet 2B fromwater by cation exchange membranes, J. Membr. Sci. 309 (2008) 239–245.  L. Fan, Y. Zhou, W. Yang, G. Chen, F. Yang, Electrochemical degradation of aqueous solution of Amaranth azo dye on ACF under potentiostatic model, Dyes Pigments 76 (2008) 440–446.  M.X. Zhu, L. Lee, H.H. Wang, Z. Wang, Removal of an anionic dye by adsorption/precipitation processes using alkaline white mud, J. Hazard. Mater. 149 (2007) 735–741.  G. Sudarjanto, B. Keller-Lehmann, J. Keller, Optimization of integrated chemical–biological degradation of a reactive azo dye using response surface methodology, J. Hazard. Mater. 138 (2006) 160–168.  V. Sarria, M. Deront, P. Peringer, C. Pulgarin, Degradation of a biorecalcitrant dye precursor present in industrial wastewaters by a new integrated iron (III) photoassisted-biological treatment, Appl. Catal. B40 (2003) 231–246.  J. Garcıa-Montano, L. Perez-Estrada, I. Oller, M.I. Maldonado, F. Torrades, J. Peral, Pilot plant scale reactive dyes degradation by solar photo-Fenton and biological processes, J. Photochem. Photobiol. A 195 (2008) 205–214.  B. Lodha, S. Chaudhari, Optimization of Fenton-biological treatment scheme for the treatment of aqueous dye solutions, J. Hazard. Mater. 148 (2007) 459–466.  B.H. Hameed, F.B.M. Daud, Adsorption studies of basic dye on activated carbon derived from agricultural waste: Hevea brasiliensis seed coat, Chem. Eng. J. 139 (2008) 48–55.  F.C. Wu, R.L. Tseng, High adsorption capacity NaOH-activated carbon for dye removal from aqueous solution, J. Hazard. Mater. 152 (2008) 1256–1267.  E. Forgacs, T. Cserhati, G. Oros, Removal of synthetic dyes from wastewaters: a review, Environ. Int. 30 (2004) 953–971.  D. Pokhrel, T. Viraraghavan, Treatment of pulp and paper mill wastewater—a review, Sci. Total Environ. 333 (2004) 37–58.  Y.M. Slokar, A. Majcen Le Marechal, Methods of decoloration of textile wastewaters, Dyes Pigments 37 (1998) 335–356.  W. Delee, O.C. Neill, F.R. Hawkes, H.M. Pinheiro, Anaerobic treatment of textile efﬂuents: a review, J. Chem. Technol. Biotechnol. 73 (1998) 323–335.  P. Cooper, Removing color from dye house waste waters: a critical review of technology available, J. Soc. Dyers Colourists 109 (1993) 97–100.  G. Crini, Non-conventional low-cost adsorbents for dye removal: a review, Bioresour. Technol. 97 (2006) 1061–1085.  V.K. Gupta, Suhas, Application of low-cost adsorbents for dye removal—a review, J. Environ. Manage. 90 (2009) 2313–2342.
Mohd. Rafatullah et al. / Journal of Hazardous Materials 177 (2010) 70–80
 Z. Aksu, Application of biosorption for the removal of organic pollutants: a review, Proc. Biochem. 40 (2005) 997–1026.  D. Wesenberg, I. Kyriakides, S.N. Agathos, White-rot fungi and their enzymes for the treatment of industrial dye efﬂuents, Biotechnol. Adv. 22 (2003) 161–187.  Y. Fu, T. Viraraghavan, Fungal decolorization of dye wastewaters: a review, Bioresour. Technol. 79 (2001) 251–262.  A. Stolz, Basic and applied aspects in the microbial degradation of azo dyes, Appl. Microbiol. Biotechnol. 56 (2001) 69–80.  A. Dabrowski, Adsorption, from theory to practice, Adv. Colloid Interface Sci. 93 (2001) 135–224.  A. Ahmad, M. Rafatullah, M. Danish, Removal of Zn(II) and Cd(II) ions from aqueous solutions using treated sawdust of sissoo wood as an adsorbent, Holz als Roh-und Werkstoff 65 (2007) 429–436.  A. Ahmad, M. Rafatullah, O. Sulaiman, M.H. Ibrahim, Y.Y. Chii, B.M. Siddique, Removal of Cu(II) and Pb(II) ions from aqueous solutions by adsorption on sawdust of Meranti wood, Desalination 247 (2009) 636–646.  M. Rafatullah, O. Sulaiman, R. Hashim, A. Ahmad, Adsorption of copper (II), chromium (III), nickel (II) and lead (II) ions from aqueous solutions by meranti sawdust, J. Hazard. Mater. 170 (2009) 969–977.  E.N. El Qada, S.J. Allen, G.M. Walker, Adsorption of basic dyes from aqueous solution onto activated carbons, Chem. Eng. J. 135 (2008) 174–184.  G.G. Stavropoulos, A.A. Zabaniotou, Production and characterization of activated carbons from olive-seed waste residue, Microporous Mesoporous Mater. 82 (2005) 79–85.  B. Bestani, N. Benderdouche, B. Benstaali, M. Belhakem, A. Addou, Methylene blue and iodine adsorption onto an activated desert plant, Bioresour. Technol. 99 (2008) 8441–8444.  M.J. Iqbal, M.N. Ashiq, Adsorption of dyes from aqueous solutions on activated charcoal, J. Hazard. Mater. B139 (2007) 57–66.  N. Kannan, M.M. Sundaram, Kinetics and mechanism of removal of methylene blue by adsorption on various carbons—a comparative study, Dyes Pigments 51 (2001) 25–40.  K.V. Kumar, S. Sivanesan, Equilibrium data, isotherm parameters and process design for partial and complete isotherm of methylene blue onto activated carbon, J. Hazard. Mater. 134 (2006) 237–244.  A.N. Fernandes, C.A.P. Almeida, C.T.B. Menezes, N.A. Debacher, M.M.D. Sierra, Removal of methylene blue from aqueous solution by peat, J. Hazard. Mater. 144 (2007) 412–419.  F. Raposo, M.A. De La Rubia, R. Borja, Methylene blue number as useful indicator to evaluate the adsorptive capacity of granular activated carbon in batch mode: inﬂuence of adsorbate/adsorbent mass ratio and particle size, J. Hazard. Mater. 165 (2009) 291–299.  V.V. Basava Rao, S.R. Mohan Rao, Adsorption studies on treatment of textile dyeing industrial efﬂuent by ﬂy ash, Chem. Eng. J. 116 (2006) 77–84.  K. Marungrueng, P. Pavasant, High performance biosorbent (Caulerpa lentillifera) for basic dye removal, Bioresour. Technol. 98 (2007) 1567– 1572.  S. Karaca, A. Gurses, R. Bayrak, Effect of some pretreatments on the adsorption of methylene blue by Balkaya lignite, Energy Convers. Manage. 45 (2004) 1693–1704.  H. Tamai, T. Kakii, Y. Hirota, T. Kumamoto, H. Yasuda, Synthesis of extremely large mesoporous activated carbon and its unique adsorption for giant molecules, Chem. Mater. 8 (1996) 454–462.  F. Banat, S. Al-Asheh, R. Al-Ahmad, F. Bni-Khalid, Bench-scale and packed bed sorption of methylene blue using treated olive pomace and charcoal, Bioresour. Technol. 98 (2007) 3017–3025.  G. McKay, G. Ramprasad, P. Pratapamowli, Equilibrium studies for the adsorption of dyestuffs from aqueous solution by low-cost materials, Water Air Soil Pollut. 29 (1986) 273–283.  G. McKay, J.F. Porter, G.R. Prasad, The removal of dye colours from aqueous solutions by adsorption on low-cost materials, Water Air Soil Pollut. 114 (1999) 423–438.  F. Banat, S. Al-Asheh, L. Al-Makhadmeh, Evaluation of the use of raw and activated date pits as potential adsorbents for dye containing waters, Process Biochem. 39 (2003) 193–202.  M. Alaya, M. Hourieh, A. Youssef, F. El-Sejarah, Adsorption properties of activated carbons prepared from olive stones by chemical and physical activation, Adsorp. Sci. Technol. 18 (1999) 27–42.  C. Saniz-Diaz, A. Grifﬁths, Activated carbon from solid wastes using a pilotscale batch ﬂaming pyrolyser, Fuel 79 (2000) 1863–1871.  Y. Lin, H. Teng, Mesoporous carbons from waste tire char and their application in wastewater discoloration, Microporous Mesoporous Mater. 54 (2002) 167–174.  B.H. Hameed, A.T.M. Din, A.L. Ahmad, Adsorption of methylene blue onto bamboo-based activated carbon: kinetics and equilibrium studies, J. Hazard. Mater. 141 (2007) 819–825.  J. Yamashita, M. Shioya, T. Kikutani, T. Hashimoto, Activated carbon ﬁbers and ﬁlms derived from poly(vinylidene ﬂuoride), Carbon 39 (2001) 207– 214.  S. Senthilkumaar, P.R. Varadarajan, K. Porkodi, C.V. Subbhuraam, Adsorption of methylene blue onto jute ﬁber carbon: kinetics and equilibrium studies, J. Colloid Interface Sci. 284 (2005) 78–82.  C. Yan, C. Wang, J. Yao, L. Zhang, X. Liu, Adsorption of methylene blue on mesoporous carbons prepared using acid- and alkaline-treated zeolite X as the template, Colloids Surf. A 333 (2009) 115–119.
 I.A.W. Tan, B.H. Hameed, A.L. Ahmad, Equilibrium and kinetic studies on basic dye adsorption by oil palm ﬁbre activated carbon, Chem. Eng. J. 127 (2007) 111–119.  B.H. Hameed, I.A.W. Tan, A.L. Ahmad, Optimization of basic dye removal by oil palm ﬁbre-based activated carbon using response surface methodology, J. Hazard. Mater. 158 (2008) 324–332.  C.A. Basar, Applicability of the various adsorption models of three dyes adsorption onto activated carbon prepared waste apricot, J. Hazard. Mater. B135 (2006) 232–241.  R.L. Tseng, S.K. Tseng, F.C. Wu, Preparation of high surface area carbons from corncob using KOH combined with CO2 gasiﬁcation for the adsorption of dyes and phenols from water, Colloids Surf. A 279 (2006) 69–78.  D. Kavitha, C. Namasivayam, Experimental and kinetic studies on methylene blue adsorption by coir pith carbon, Bioresour. Technol. 98 (2007) 14–21.  B.H. Hameed, A.L. Ahmad, K.N.A. Latiff, Adsorption of basic dye (methylene blue) onto activated carbon prepared from rattan sawdust, Dyes Pigments 75 (2007) 143–149.  O. Gercel, A. Ozcan, A.S. Ozcan, H.F. Gercel, Preparation of activated carbon from a renewable bio-plant of Euphorbia rigida by H2 SO4 activation and its adsorption behavior in aqueous solutions, Appl. Surf. Sci. 253 (2007) 4843–4852.  S. Altenor, B. Carene, E. Emmanuel, J. Lambert, J.J. Ehrhardt, S. Gaspard, Adsorption studies of methylene blue and phenol onto vetiver roots activated carbon prepared by chemical activation, J. Hazard. Mater. 165 (2009) 1029–1039.  T.C. Chandra, M.M. Mirna, Y. Sudaryanto, S. Ismadji, Adsorption of basic dye onto activated carbon prepared from durian shell: studies of adsorption equilibrium and kinetics, Chem. Eng. J. 127 (2007) 121–129.  K. Legrouri, E. Khouyab, M. Ezzinea, H. Hannachea, R. Denoyelc, R. Pallierd, R. Naslaind, Production of activated carbon from a new precursor molasses by activation with sulphuric acid, J. Hazard. Mater. B118 (2005) 259–263.  A. Ozer, G. Dursun, Removal of methylene blue from aqueous solution by dehydrated wheat bran carbon, J. Hazard. Mater. 146 (2007) 262–269.  A.A. Attia, B.S. Girgis, N.A. Fathy, Removal of methylene blue by carbons derived from peach stones by H3 PO4 activation: batch and column studies, Dyes Pigments 76 (2008) 282–289.  A. Aygun, S. Yenisoy-Karakas, I. Duman, Production of granular activated carbon from fruit stones and nutshells and evaluation of their physical, chemical and adsorption properties, Microporous Mesoporous Mater. 66 (2003) 189–195.  A. Gurses, C. Dogar, S. Karaca, M. Acikyildiz, R. Bayrak, Production of granular activated carbon from waste Rosa canina sp. seeds and its adsorption characteristics for dye, J. Hazard. Mater. B131 (2006) 254–259.  Y. Guo, S. Yang, W. Fu, J. Qi, R. Li, Z. Wang, H. Xu, Adsorption of malachite green on micro- and mesoporous rice husk-based active carbon, Dyes Pigments 56 (2003) 219–229.  S.E. Bailey, T.J. Olin, M. Bricka, D.D. Adrian, A review of potentially low-cost sorbents for heavy metals, Water Res. 33 (1999) 2469–2479.  T. Pinnavaia, Intercalated clay catalysts, J. Sci. 220 (4595) (1983) 365–371.  K.G. Bhattacharyya, S.S. Gupta, adsorption of a few heavy metals on natural and modiﬁed kaolinite and montmorillonite: a review, Adv. Colloid Interface Sci. 140 (2008) 114–131.  S. Babel, T.A. Kurniawan, Low-cost adsorbents for heavy metals uptake from contaminated water: a review, J. Hazard. Mater. B97 (2003) 219–243.  G. McKay, V. Poots, Kinetics and diffusion processes in color removal from efﬂuent using wood, J. Chem. Technol. Biotechnol. 30 (1986) 279–282.  G. Atun, G. Hisarli, W.S. Sheldrick, M. Muhler, Adsorptive removal of methylene blue from colored efﬂuents on fuller’s earth, J. Colloid Interface Sci. 261 (2003) 32–39.  S. Hong, C. Wen, J. He, F. Gan, Y.S. Ho, Adsorption thermodynamics of methylene blue onto bentonite, J. Hazard. Mater. 167 (2009) 630–633.  A. Gurses, S. Karaca, C. Dogar, R. Bayrak, M. Ac¸ıkyıldız, M. Yalc¸ın, Determination of adsorptive properties of clay/water system: methylene blue sorption, J. Colloid Interface Sci. 269 (2004) 310–314.  R.A. Shawabkeh, M.F. Tutunji, Experimental study and modelling of basic dye sorption by diatomaceous clay, Appl. Clay Sci. 24 (2003) 111–120.  A. Gucek, S. S¸ener, S. Bilgen, M.A. Mazmancı, Adsorption and kinetic studies of cationic and anionic dyes on pyrophyllite from aqueous solutions, J. Colloid Interface Sci. 286 (2005) 53–60.  M. Hajjaji, A. Alami, A. El Bouadili, Removal of methylene blue from aqueous solution by ﬁbrous clay minerals, J. Hazard. Mater. B135 (2006) 188–192.  C.A.P. Almeida, N.A. Debacher, A.J. Downs, L. Cottet, C.A.D. Mello, Removal of methylene blue from colored efﬂuents by adsorption on montmorillonite clay, J. Colloid Interface Sci. 332 (2009) 46–53.  A. Al-Futaisi, A. Jamrah, R. Al-Hanai, Aspects of cationic dye molecule adsorption to palygorskite, Desalination 214 (2007) 327–342.  M. Bagane, S. Guiza, Removal of a dye from textile efﬂuents by adsorption, Ann. Chim. 25 (2000) 615–626.  M.A. Al-Ghouti, M.A.M. Khraisheh, S.J. Allen, M.N. Ahmad, The removal of dyes from textile wastewater: a study of the physical characteristics and adsorption mechanisms of diatomaceous earth, J. Environ. Manage. 69 (2003) 229–238.  C.H. Weng, Y.F. Pan, Adsorption of a cationic dye (methylene blue) onto spent activated clay, J. Hazard. Mater. 144 (2007) 355–362.  C.K. Lee, K.S. Low, L.C. Chung, Removal of some organic dyes by hexaneextracted spent bleaching earth, J. Chem. Technol. Biotechnol. 69 (1997) 93–99.
Mohd. Rafatullah et al. / Journal of Hazardous Materials 177 (2010) 70–80  C. Woolard, J. Strong, C. Erasmus, Evaluation of the use of modiﬁed coal ash as a potential sorbent for organic waste streams, Appl. Geochem. 17 (2002) 1159–1164.  M.N. Ahmed, R.N. Ram, Removal of basic dye from wastewater using silica as adsorbent, Environ. Pollut. 77 (1992) 79–86.  M. Dogan, M. Alkan, Y. Onager, Adsorption of methylene blue from aqueous solution onto perlite, Water Air Soil Pollut. 120 (2000) 229–248.  M. Dogan, M. Alkan, A. Turkyilmaz, Y. Ozdemir, Kinetics and mechanism of removal of methylene blue by adsorption onto perlite, J. Hazard. Mater. B109 (2004) 141–148.  S. Chakrabarti, B.K. Dutta, Note on the adsorption and diffusion of methylene blue in glass ﬁbers, J. Colloid Interface Sci. 286 (2005) 807–811.  H. Ghobarkar, O. Schaf, U. Guth, Zeolites—from kitchen to space, Prog. Solid State Chem. 27 (1999) 29–73.  J.X. Yu, B.H. Li, X.M. Sun, J. Yuan, R.A. Chi, Polymer modiﬁed biomass of baker’s yeast for enhancement adsorption of methylene blue, rhodamine B and basic magenta, J. Hazard. Mater. 168 (2009) 1147–1154.  J.X. Yu, B.H. Li, X.M. Sun, J. Yuan, R.A. Chi, Poly(amic acid)-modiﬁed biomass of baker’s yeast for enhancement adsorption of methylene blue and basic magenta, Appl. Biochem. Biotechnol. (2009), doi:10.1007/s12010-009-86014.  E. Rubin, P. Rodriguez, R. Herrero, J. Cremades, I. Barbara, M.E. Sastre de Vicente, Removal of methylene blue from aqueous solutions using as biosorbent Sargassum muticum: an invasive macroalga in Europe, J. Chem. Technol. Biotechnol. 80 (2005) 291–298.  O. Gulnaz, A. Kaya, F. Matyar, B. Arikan, Sorption of basic dyes from aqueous solution by activated sludge, J. Hazard. Mater. B108 (2004) 183–188.  K.S. Low, C.K. Lee, L.L. Heng, Sorption of basic dyes by Hydrilla verticillata, Environ. Technol. 14 (1993) 115–124.  K.S. Low, C.K. Lee, K.K. Tan, Biosorption of basic dyes by water hyacinth roots, Bioresour. Technol. 52 (1995) 79–83.  V.J.P. Vilar, C.M.S. Botelho, R.A.R. Boaventura, Methylene blue adsorption by algal biomass based materials: biosorbents characterization and process behaviour, J. Hazard. Mater. 147 (2007) 120–132.  P. Waranusantigul, P. Pokethitiyook, M. Kruatrachue, E.S. Upatham, Kinetics of basic dye (Methylene Blue) biosorption by giant duckweed (Spirodela polyrrhiza), Environ. Pollut. 125 (2003) 385–392.  N.S. Maurya, A.K. Mittal, P. Cornel, E. Rother, Biosorption of dyes using dead macro fungi: effect of dye structure, ionic strength and pH, Bioresour. Technol. 97 (2006) 512–521.  D. Caparkaya, L. Cavas, Biosorption of methylene blue by a brown alga Cystoseira barbatula Kützing, Acta Chim. Slov. 55 (2008) 547–553.  Y. Nacera, B. Aicha, Equilibrium and kinetic modelling of methylene blue biosorption by pretreated dead Streptomyces rimosus: effect of temperature, Chem. Eng. J. 119 (2006) 121–125.  Y. Fu, T. Viraraghavan, Removal of a dye from an aqueous solution by the fungus Aspergillus niger, Water Qual. Res. J. Can. 35 (1) (2000) 95–111.  M.C. Ncibi, B. Mahjoub, M. Seffen, Kinetic and equilibrium studies of methylene blue biosorption by Posidonia oceanica (L.) ﬁbres, J. Hazard. Mater. 139 (2007) 280–285.  M.C. Ncibi, A.M.B. Hamissa, A. Fathallah, M.H. Kortas, T. Baklouti, B. Mahjoub, M. Seffen, Biosorptive uptake of methylene blue using Mediterranean green alga Enteromorpha spp., J. Hazard. Mater. 170 (2009) 1050–1055.  S. Cengiz, L. Cavas, Removal of methylene blue by invasive marine seaweed: Caulerpa racemosa var. cylindracea, Bioresour. Technol. 99 (2008) 2357– 2363.  A. El Sikaily, A. Khaled, A. El Nemr, O. Abdelwahab, Removal of methylene blue from aqueous solution by marine green alga Ulva lactuca, Chem. Ecol. 22 (2) (2006) 149–157.  M.I. El-Khaiary, Kinetics and mechanism of adsorption of methylene blue from aqueous solution by nitric-acid treated water-hyacinth, J. Hazard. Mater. 147 (2007) 28–36.  V.K. Garg, M. Amita, R. Kumar, R. Gupta, Basic dye (methylene blue) removal from simulated wastewater by adsorption using Indian Rosewood sawdust: a timber industry waste, Dyes Pigments 63 (2004) 243–250.  A. Shukla, Y. Zhang, P. Dubey, J.L. Margrave, S.S. Shukla, The role of sawdust in the removal of unwanted materials from water, J. Hazard. Mater. B95 (2002) 137–152.  O. Hamdaoui, Batch study of liquid-phase adsorption of methylene blue using cedar sawdust and crushed brick, J. Hazard. Mater. B135 (2006) 264–273.  A. Ahmad, M. Rafatullah, O. Sulaiman, M.H. Ibrahim, R. Hashim, Scavenging behaviour of meranti sawdust in the removal of methylene blue from aqueous solution, J. Hazard. Mater. 170 (2009) 357–365.  S. Chakraborty, S. De, S. Dasgupta, J.K. Basu, Removal of dyes from aqueous solution using a low cost adsorbent, in: Water and Wastewater Perspectives of Developing Countries, Proceedings of International Conference, International Water Association, New Delhi, India, 2002, pp. 1089–1096.  F. Ferrero, Dye removal by low cost adsorbents: hazelnut shells in comparison with wood sawdust, J. Hazard. Mater. 142 (2007) 144–152.  A.E. Ofomaja, Equilibrium sorption of methylene blue using mansonia wood sawdust as biosorbents, Desalination Water Treat. 3 (2009) 1–10.  D.S. De, J.K. Basu, Adsorption of methylene blue on to a low cost adsorbent developed from sawdust, Ind. J. Environ. Protec. 19 (1998) 416–421.  P. Janos, S. Coskun, V. Pilarová, J. Rejnek, Removal of basic (Methylene Blue) and acid (Egacid Orange) dyes from waters by sorption on chemically treated wood shavings, Bioresour. Technol. 100 (2009) 1450–1453.
 F.A. Batzias, D.K. Sidiras, Dye adsorption by calcium chloride treated beech sawdust in batch and ﬁxed-bed systems, J. Hazard. Mater. B114 (2004) 167–174.  F.A. Batzias, D.K. Sidiras, Dye adsorption by prehydrolysed beech sawdust in batch and ﬁxed-bed systems, Bioresour. Technol. 98 (2007) 1208–1217.  F.A. Batzias, D.K. Sidiras, Simulation of dye adsorption by beech sawdust as affected by pH, J. Hazard. Mater. 141 (2007) 668–679.  P.T. Williams, N. Nugranad, Comparison of products from the pyrolysis and catalytic pyrolysis of rice husks, Energy 25 (2000) 493–513.  V. Vadivelan, K.V. Kumar, Equilibrium, kinetics, mechanism, and process design for the sorption of methylene blue onto rice husk, J. Colloid Interface Sci. 286 (2005) 90–100.  B.H. Hameed, Evaluation of papaya seeds as a novel non-conventional lowcost adsorbent for removal of methylene blue, J. Hazard. Mater. 162 (2009) 939–944.  B.H. Hameed, Grass waste: a novel sorbent for the removal of basic dye from aqueous solution, J. Hazard. Mater. 166 (2009) 233–238.  K.V. Kumar, K. Porkodi, Mass transfer, kinetics and equilibrium studies for the biosorption of methylene blue using Paspalum notatum, J. Hazard. Mater. 146 (2007) 214–226.  B.H. Hameed, D.K. Mahmoud, A.L. Ahmad, Sorption of basic dye from aqueous solution by pomelo (Citrus grandis) peel in a batch system, Colloids Surf. A316 (2008) 78–84.  V. Ponnusami, S. Vikram, S.N. Srivastava, Guava (Psidium guajava) leaf powder: novel adsorbent for removal of methylene blue from aqueous solutions, J. Hazard. Mater. 152 (2008) 276–286.  D.K. Singh, B. Srivastava, Removal of basic dyes from aqueous solutions by chemically treated Psidium guyava leaves, Indian J. Environ. Health 41 (1999) 333–345.  V. Ponnusami, V. Gunasekar, S.N. Srivastava, Kinetics of methylene blue removal from aqueous solution using gulmohar (Delonix regia) plant leaf powder: multivariate regression analysis, J. Hazard. Mater. 169 (2009) 119– 127.  B.H. Hameed, Removal of cationic dye from aqueous solution using jackfruit peel as non-conventional low-cost adsorbent, J. Hazard. Mater. 162 (2009) 344–350.  B.H. Hameed, D.K. Mahmoud, A.L. Ahmad, Sorption equilibrium and kinetics of basic dye from aqueous solution using banana stalk waste, J. Hazard. Mater. 158 (2008) 499–506.  G. Annadurai, R. Juang, D. Lee, Use of cellulose-based wastes for adsorption of dyes from aqueous solutions, J. Hazard. Mater. B92 (2002) 263–274.  A.E. Ofomaja, Sorption dynamics and isotherm studies of methylene blue uptake on to palm kernel ﬁbre, Chem. Eng. J. 126 (2007) 35–43.  R. Gong, Y. Jin, J. Chen, Y. Hu, J. Sun, Removal of basic dyes from aqueous solution by sorption on phosphoric acid modiﬁed rice straw, Dyes Pigments 73 (2007) 332–337.  B.H. Hameed, M.I. El-Khaiary, Sorption kinetics and isotherm studies of a cationic dye using agricultural waste: broad bean peels, J. Hazard. Mater. 154 (2008) 639–648.  N.A. Oladoja, I.O. Asia, C.O. Aboluwoye, Y.B. Oladimeji, A.O. Ashogbon, Studies on the sorption of basic dye by rubber (Hevea brasiliensis) seed shell, Turk. J. Eng. Environ. Sci. 32 (2008) 143–152.  N.A. Oladoja, C.O. Aboluwoye, Y.B. Oladimeji, A.O. Ashogbon, I.O. Otemuyiwa, Studies on castor seed shell as a sorbent in basic dye contaminated wastewater remediation, Desalination 227 (2008) 190–203.  B.H. Hameed, M.I. El-Khaiary, Removal of basic dye from aqueous medium using a novel agricultural waste material: pumpkin seed hull, J. Hazard. Mater. 155 (2008) 601–609.  B.H. Hameed, R.R. Krishni, S.A. Sata, A novel agricultural waste adsorbent for the removal of cationic dye from aqueous solutions, J. Hazard. Mater. 162 (2009) 305–311.  D. Ozer, G. Dursun, A. Ozer, Methylene blue adsorption from aqueous solution by dehydrated peanut hull, J. Hazard. Mater. 144 (2007) 171–179.  K.S. Low, C.K. Lee, The removal of cationic dyes using coconut husk as an absorbent, Pertanika 13 (1990) 221–228.  L.S. Oliveira, A.S. Franca, T.M. Alves, S.D.F. Rocha, Evaluation of untreated coffee husks as potential biosorbents for treatment of dye contaminated waters, J. Hazard. Mater. 155 (2008) 507–512.  H. Lata, V.K. Garg, R.K. Gupta, Removal of a basic dye from aqueous solution by adsorption using Parthenium hysterophorus: an agricultural waste, Dyes Pigments 74 (2007) 653–658.  B.H. Hameed, A.A. Ahmad, Batch adsorption of methylene blue from aqueous solution by garlic peel, an agricultural waste biomass, J. Hazard. Mater. 164 (2009) 870–875.  R. Han, W. Zou, W. Yu, S. Cheng, Y. Wang, J. Shi, Biosorption of methylene blue from aqueous solution by fallen phoenix tree’s leaves, J. Hazard. Mater. 141 (2007) 156–162.  M. Dogan, H. Abak, M. Alkan, Biosorption of methylene blue from aqueous solutions by hazelnut shells: equilibrium, parameters and isotherms, Water Air Soil Pollut. 192 (2008) 141–153.  M. Dogan, H. Abak, M. Alkan, Adsorption of methylene blue onto hazelnut shell: kinetics, mechanism and activation parameters, J. Hazard. Mater. 164 (2009) 172–181.  B.H. Hameed, D.K. Mahmoud, A.L. Ahmad, Equilibrium modeling and kinetic studies on the adsorption of basic dye by a low-cost adsorbent: coconut (Cocos nucifera) bunch waste, J. Hazard. Mater. 158 (2008) 65–72.
Mohd. Rafatullah et al. / Journal of Hazardous Materials 177 (2010) 70–80
 R. Gong, M. Li, C. Yang, Y. Sun, J. Chen, Removal of cationic dyes from aqueous solution by adsorption on peanut hull, J. Hazard. Mater. B121 (2005) 247–250.  H. Demir, A. Top, D. Balkose, S. Ulku, Dye adsorption behavior of Luffa cylindrica ﬁbers, J. Hazard. Mater. 153 (2008) 389–394.  F.A. Pavan, E.C. Lima, S.L.P. Dias, A.C. Mazzocato, Methylene blue biosorption from aqueous solutions by yellow passion fruit waste, J. Hazard. Mater. 150 (2008) 703–712.  S. Banerjee, M.G. Dastidar, Use of jute processing wastes for treatment of wastewater contaminated with dye and other organics, Bioresour. Technol. 96 (2005) 1919–1928.  R. Han, Y. Wang, P. Han, J. Shi, J. Yang, Y. Lu, Removal of methylene blue from aqueous solution by chaff in batch mode, J. Hazard. Mater. B137 (2006) 550–557.  Y. Bulut, H.A. Aydin, Kinetics and thermodynamics study of methylene blue adsorption on wheat shells, Desalination 194 (2006) 259–267.  F.A. Batzias, D.K. Sidiras, E. Schroeder, C. Weber, Simulation of dye adsorption on hydrolyzed wheat straw in batch and ﬁxed-bed systems, Chem. Eng. J. 148 (2009) 459–472.  K.G. Bhattacharyya, A. Sharma, Kinetics and thermodynamics of methylene blue adsorption on neem (Azadirachta indica) leaf powder, Dyes Pigments 65 (2005) 51–59.  M. Otero, F. Rozada, L.F. Calvo, A.I. Garcia, A. Moran, Kinetic and equilibrium modelling of the methylene blue removal from solution by adsorbent materials produced from sewage sludges, Biochem. Eng. J. 15 (2003) 59–68.  C. Lee, K. Low, S. Chow, Chrome sludge as an adsorbent for color removal, Environ. Technol. 54 (1996) 183–189.  S. Wang, Y. Boyjoo, A.A. Choueib, Comparative study of dye removal using ﬂy ash treated by different methods, Chemosphere 60 (2005) 1401–1407.  S. Wang, Q. Ma, Z.H. Zhu, Characteristics of coal ﬂy ash and adsorption application, Fuel 87 (2008) 3469–3473.  V.K. Gupta, D. Mohan, S. Sharma, M. Sharma, Removal of basic dyes (rhodamine B and methylene blue) from aqueous solutions using baggase ﬂy ash, Sep. Sci. Technol. 35 (2000) 2097–2113.
 T. Viraraghavan, K.R. Ramakrishna, Fly ash for colour removal from synthetic dye solutions, Water Qual. Res. J. Can. 34 (1999) 505–517.  P. Janos, H. Buchtova, M. Ryznarova, Sorption of dyes from aqueous solution onto ﬂy ash, Water Res. 37 (2003) 4938–4944.  K.V. Kumar, V. Ramamurthi, S. Sivanesan, Modeling the mechanism involved during the sorption of methylene blue onto ﬂy ash, J. Colloid Interface Sci. 284 (2005) 14–21.  M.T. Uddin, M.A. Islam, S. Mahmud, M. Rukanuzzaman, Adsorptive removal of methylene blue by tea waste, J. Hazard. Mater. 164 (2009) 53–60.  B.H. Hameed, Spent tea leaves: a new non-conventional and low-cost adsorbent for removal of basic dye from aqueous solutions, J. Hazard. Mater. 161 (2009) 753–759.  B.B. Saeed, M.A. Rauf, S.S. AlAli, Removal of methylene blue from aqueous solution by adsorption on sand, Dyes Pigments 74 (2007) 85–87.  K. Imamura, E. Ikeda, T. Nagayasu, T. Sakiyama, K. Nakanishi, Adsorption behavior of methylene blue and its congeners on a stainless steel surface, J. Colloid Interface Sci. 245 (2002) 50–57.  K.V. Kumar, Adsorption isotherm for basic dye onto low cost adsorbents, Res. J. Chem. Environ. 6 (4) (2002) 61–65.  A. Namasivayam, S. Sumithra, Removal of direct red 12B and methylene blue from water by adsorption onto Fe(III)/Cr(III) hydroxide, an industrial solid waste, J. Environ. Manage. 74 (2005) 207–215.  F.A. Ozdemir, B. Demirata, R. Apak, Adsorptive removal of methylene blue from simulated dyeing wastewater with melamine–formaldehyde–urea resin, J. Appl. Polym. Sci. 112 (2009) 3442–3448.  W.T. Tsai, J.M. Yang, C.W. Lai, Y.H. Cheng, C.C. Lin, C.W. Yeh, Characterization and adsorption properties of eggshells and eggshell membrane, Bioresour. Technol. 97 (3) (2006) 488–493.  S.Y. Mak, D.H. Chen, Fast adsorption of methylene blue on polyacrylic acidbound iron oxide magnetic nanoparticles, Dyes Pigments 61 (2004) 93– 98.